The article presents crystallization process of silicon molybdenum ductile cast iron (SiMo). The alloy with 5% silicon content and with variable amounts of Mo in a range of 0-1% was chosen for the research. The carbon content in the analysed alloys did not exceed 3,1%. The studies of crystallization process were based on thermal – derivative analysis (TDA). Chemical composition of all examined samples was analysed with the use of LECO spectrometer. Additionally, the carbon and the sulphur content was determined basing on carbon and sulphur LECO analyser. For metallographic examination, the scanning electron microscopy (SEM) with EDS analyser was used. Disclosed phases have been also tested with the use of X-ray diffraction. The results allowed the description of crystallization processes of silicon molybdenum ductile cast iron using thermal – derivative analysis (TDA). Conducted studies did not allow for the clear identification of all complex phases containing molybdenum, occurring at the grain boundaries. Therefore, the further stages of the research could include the use of a transmission electron microscope to specify the description of complex compounds present in the alloy.
In the dissertation it has been shown, that so called “time-thermal treatment” (TTT) of the alloy in liquid state as overheating the metal with around 250o C above Tliq. and detailing it in temperature for 30 to 40 minutes has the influence on changing the crystallization parameters (Tliq., TEmin. , TEmax., TE(Me), TSol.). It was ascertained, that overheating the AlSi17Cu5Mg alloy substantially above Tliq. results with microcrystalline structure. Evenly distributed in the eutectic warp primeval silicon crystals and supersaturated with alloying additives of base content (Cu, Mg, Fe) of α(Al) solution, ensures not only increase durability in ambient temperature, but also at elevated temperature (250o C), what due to it’s use in car industry is an advantage.
The modification is a widespread method of improving the strength properties of cast iron. The impact in terms of increasing amounts of eutectic grains has been thoroughly studied while the issue of the impact on the mechanical properties of primary austenite grains has not been studied in depth yet. The paper presents the study of both aspects. The methodology was to conduct the melting cast iron with flake graphite, then modifying the alloy by two sets of modifiers: the commercial modifier, and a mixture of iron powder with a commercial inoculant. The DAAS test was carried out to identify the primary austenite grains. The degree of supercooling was determined and the UTS test was performed as well. Additionally carried out the metallographic specimen allowing for counting grains. It can be concluded that the introduction of the iron powder significantly improved the number of austenite primary grains which resulted in an increase in tensile strength UTS.
Particles of the Fe-Al type (less than 50 µm in diameter) were sprayed onto the 045 steel substrate by means of the detonation method. The TEM, SAED and EDX analyses revealed that the Fe-Al particles have been partially melted in the experiment of coating formation. Particle undergone melting even within about 80% of its volume. Therefore, solidification of the melted part of particles was expected. Solidification differed significantly due to a large range of chemical composition of applied particles (from 15 at.% Al up to 63 at.% Al). A single particle containing 63 at.% Al was subjected to the detailed analysis, only. The TEM / SAED techniques revealed in the solidified part of particle three sub-layers: an amorphous phase, A ε , periodically situated FeAl + Fe2Al5 phases, and a non-equilibrium phase, Nε . A hypothesis dealing with the inter-metallic phases formation in such a single particle of the nominal composition 0 N = 0.63 is presented. At first, the solid / liquid system is treated as an interconnection: substrate liquid nonmelted particle part / / . Therefore, it is suggested that the solidification occurs simultaneously in two directions: towards a substrate and towards a non-melted part of particle. The solidification mechanism is referred to the Fe-Al meta-stable phase diagram. It is shown that the melted part of particle solidifies rapidly according to the phase diagram of meta-stable equilibrium and at a significant deviation from the thermodynamic equilibrium.
The paper concerns experimental work studying chemical composition, structures and selected mechanical properties of castings produced by rheocasting method SEED. After previous experiments, which showed inclusions in the primary phase α(Al) when observing structures, hypothesis of external nuclei was taken. The main goal of the work was to determine the influence of inoculation by various additions of titanium/boron based inoculant on the structure and properties of AlSi7Mg0,3 alloy. The master alloy AlTi5B1 was added in amounts of 0,05, 0,1, 0,15, 0,2 wt %. Metallographic observation by light and SEM microscopy was used for analysing the structures. Measurements of grain size were realised and evaluated. Brinell hardness measurements were performed. Chemical composition was measured by GDS analysis. Undertaken experiments did not prove the effect of inoculation of combined AlTi5B1 master alloy on castings made of AlSi7Mg0,3 alloy made by rheocasting SEED at given amounts and conditions.